Question 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm


 Jasmine Jones
 2 years ago
 Views:
Transcription
1 14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation. Calculate the resulting strain. This problem calls for us to calculate the elastic strain that results for an aluminum specimen stressed in tension. The crosssectional area is just (10 mm) (12.7 mm) 127 mm 2 ( m in. 2 ); also, the elastic modulus for Al is given in Table 6.1 as 69 GPa (or N/m 2 ). Combining Equations 6.1 and 6.5 and solving for the strain yields E F A 0 E 35,500 N ( m 2 )( N/m ) Question 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm (0.8 in.) on an edge is pulled in tension with a load of 89,000 N (20,000 lb f ), and experiences an elongation of 0.10 mm ( in.). Assuming that the deformation is entirely elastic, calculate the elastic modulus of the steel. This problem asks us to compute the elastic modulus of steel. For a square crosssection, A 0 b 2 0, where b 0 is the edge length. Combining Equations 6.1, 6.2, and 6.5 and solving for E, leads to E F A 0 l l 0 Fl 0 b 0 2 l (89,000 N)( m) ( m) 2 ( m) N/m GPa ( psi)
2 Question 6.7: For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa ( psi). (a) What is the maximum load that may be applied to a specimen with a crosssectional area of 325 mm 2 (0.5 in. 2 ) without plastic deformation? (b) If the original specimen length is 115 mm (4.5 in.), what is the maximum length to which it may be stretched without causing plastic deformation? (a) This portion of the problem calls for a determination of the maximum load that can be applied without plastic deformation (F y ). Taking the yield strength to be 275 MPa, and employment of Equation 6.1 leads to F y y A 0 ( N/m 2 )( m 2 ) 89,375 N (20,000 lb f ) (b) The maximum length to which the sample may be deformed without plastic deformation is determined from Equations 6.2 and 6.5 as l i l 0 1 E 275 MPa (115 mm) mm (4.51 in.) MPa Question 6.13: In Section 2.6 it was noted that the net bonding energy E N between two isolated positive and negative ions is a function of interionic distance r as follows: E N A r B r n (6.25) where A, B, and n are constants for the particular ion pair. Equation 6.25 is also valid for the bonding energy between adjacent ions in solid materials. The modulus of elasticity E is proportional to the slope of the interionic force separation curve at the equilibrium interionic separation; that is,
3 E df dr r o Derive an expression for the dependence of the modulus of elasticity on these A, B, and n parameters (for the twoion system) using the following procedure: 1. Establish a relationship for the force F as a function of r, realizing that F de N dr 2. Now take the derivative df/dr. 3. Develop an expression for r 0, the equilibrium separation. Since r 0 corresponds to the value of r at the minimum of the E N versusr curve (Figure 2.8b), take the derivative de N /dr, set it equal to zero, and solve for r, which corresponds to r Finally, substitute this expression for r 0 into the relationship obtained by taking df/dr. This problem asks that we derive an expression for the dependence of the modulus of elasticity, E, on the parameters A, B, and n in Equation It is first necessary to take de N /dr in order to obtain an expression for the force F; this is accomplished as follows: F de N dr d A r + dr d B r n dr A r 2 nb r (n 1) The second step is to set this de N /dr expression equal to zero and then solve for r ( r 0 ). The algebra for this procedure is carried out in Problem 2.14, with the result that r 0 A 1/(1 n) nb Next it becomes necessary to take the derivative of the force (df/dr), which is accomplished as follows:
4 df dr d A r 2 + dr d nb r (n 1) dr 2 A (n)(n 1)B + r 3 r (n 2) Now, substitution of the above expression for r 0 into this equation yields df dr r 0 2A A 3/(1 n) nb + (n)(n 1) B A (n 2)/(1 n) nb which is the expression to which the modulus of elasticity is proportional. Question 6.14: Using the solution to Problem 6.13, rank the magnitudes of the moduli of elasticity for the following hypothetical X, Y, and Z materials from the greatest to the least. The appropriate A, B, and n parameters (Equation 6.25) for these three materials are tabulated below; they yield E N in units of electron volts and r in nanometers: Material A B n X Y Z This problem asks that we rank the magnitudes of the moduli of elasticity of the three hypothetical metals X, Y, and Z. From Problem 6.13, it was shown for materials in which the bonding energy is dependent on the interatomic distance r according to Equation 6.25, that the modulus of elasticity E is proportional to 2A E A 3/(1 n) nb + (n)(n 1) B A (n 2)/(1 n) nb For metal X, A 2.5, B , and n 8. Therefore,
5 (2)(2.5) E 3/(1 8) 2.5 (8)( ) + (8)(8 1)( ) (8 2)/(1 8) 2.5 (8)( ) 1097 For metal Y, A 2.3, B , and n Hence E (2)(2.3) 3/(1 10.5) 2.3 (10.5) ( ) + (10.5)(10.5 1)( ) (10.5 2)/(1 10.5) 2.3 (10.5) ( ) 551 And, for metal Z, A 3.0, B , and n 9. Thus E (2)(3.0) 3/(1 9) 3.0 (9)( ) + (9)(9 1)( ) (9 2)/(1 9) 3.0 (9)( ) 1024 Therefore, metal X has the highest modulus of elasticity. Question 15: A cylindrical specimen of aluminum having a diameter of 19 mm (0.75 in.) and length of 200 mm (8.0 in.) is deformed elastically in tension with a force of 48,800 N (11,000 lb f ). Using the data contained in Table 6.1, determine the following: (a) The amount by which this specimen will elongate in the direction of the applied stress. (b) The change in diameter of the specimen. Will the diameter increase or decrease? (a) We are asked, in this portion of the problem, to determine the elongation of a cylindrical specimen of aluminum. Combining Equations 6.1, 6.2, and 6.5, leads to
6 E F d 0 2 E l l 0 4 Or, solving for l (and realizing that E 69 GPa, Table 6.1), yields l 4Fl 0 d 0 2 E (4)(48,800 N)( m) ( )( m) 2 ( N/m 2 ) m 0.50 mm (0.02 in.) (b) We are now called upon to determine the change in diameter, d. Using Equation 6.8 x z d / d 0 l /l 0 From Table 6.1, for aluminum, Now, solving the above expression for d yields d ld 0 l 0 (0.33)(0.50 mm)(19 mm) 200 mm mm ( in.) The diameter will decrease. Question 6.20: A brass alloy is known to have a yield strength of 275 MPa (40,000 psi), a tensile strength of 380 MPa (55,000 psi), and an elastic modulus of 103 GPa ( psi). A cylindrical specimen of this alloy 12.7 mm (0.50 in.) in diameter and 250 mm (10.0 in.) long is stressed in tension and found to elongate 7.6 mm (0.30 in.). On the basis of the information given, is it possible to compute the magnitude of the load that is necessary to produce this change in length? If so, calculate the load. If not, explain why.
7 We are asked to ascertain whether or not it is possible to compute, for brass, the magnitude of the load necessary to produce an elongation of 7.6 mm (0.30 in.). It is first necessary to compute the strain at yielding from the yield strength and the elastic modulus, and then the strain experienced by the test specimen. Then, if (test) < (yield) deformation is elastic, and the load may be computed using Equations 6.1 and 6.5. However, if (test) > (yield) computation of the load is not possible inasmuch as deformation is plastic and we have neither a stressstrain plot nor a mathematical expression relating plastic stress and strain. We compute these two strain values as (test) l l mm 250 mm 0.03 and (yield) y E 275 MPa MPa Therefore, computation of the load is not possible since (test) > (yield). Question 6.22: Consider the brass alloy for which the stressstrain behavior is shown in Figure A cylindrical specimen of this material 6 mm (0.24 in.) in diameter and 50 mm (2 in.) long is pulled in tension with a force of 5000 N (1125 lb f ). If it is known that this alloy has a Poisson's ratio of 0.30, compute: (a) the specimen elongation, and (b) the reduction in specimen diameter. (a) This portion of the problem asks that we compute the elongation of the brass specimen. The first calculation necessary is that of the applied stress using Equation 6.1, as F A 0 F d N m N/m MPa (25,000 psi) 2 2
8 From the stressstrain plot in Figure 6.12, this stress corresponds to a strain of about From the definition of strain, Equation 6.2 l l 0 ( )(50 mm) 0.10 mm ( in.) (b) In order to determine the reduction in diameter d, it is necessary to use Equation 6.8 and the definition of lateral strain (i.e., x d/d 0 ) as follows d d 0 x d 0 z (6 mm)(0.30)( ) mm ( in.) Question 6.27: A load of 85,000 N (19,100 lb f ) is applied to a cylindrical specimen of a steel alloy (displaying the stress strain behavior shown in Figure 6.21) that has a crosssectional diameter of 15 mm (0.59 in.). (a) Will the specimen experience elastic and/or plastic deformation? Why? (b) If the original specimen length is 250 mm (10 in.), how much will it increase in length when this load is applied? This problem asks us to determine the deformation characteristics of a steel specimen, the stressstrain behavior for which is shown in Figure (a) In order to ascertain whether the deformation is elastic or plastic, we must first compute the stress, then locate it on the stressstrain curve, and, finally, note whether this point is on the elastic or plastic region. Thus, from Equation 6.1 F A 0 85, 000 N m N/m MPa (69,900 psi) 2 The 481 MPa point is beyond the linear portion of the curve, and, therefore, the deformation will be both elastic and plastic. (b) This portion of the problem asks us to compute the increase in specimen length. From the stressstrain curve, the strain at 481 MPa is approximately Thus, from Equation 6.2
9 l l 0 (0.0135)(250 mm) 3.4 mm (0.135 in.) Question 6.28: A bar of a steel alloy that exhibits the stressstrain behavior shown in Figure 6.21 is subjected to a tensile load; the specimen is 300 mm (12 in.) long, and of square cross section 4.5 mm (0.175 in.) on a side. (a) Compute the magnitude of the load necessary to produce an elongation of 0.45 mm (0.018 in.). (b) What will be the deformation after the load has been released? (a) We are asked to compute the magnitude of the load necessary to produce an elongation of 0.45 mm for the steel displaying the stressstrain behavior shown in Figure First, calculate the strain, and then the corresponding stress from the plot. l l mm 300 mm This is near the end of the elastic region; from the inset of Figure 6.21, this corresponds to a stress of about 300 MPa (43,500 psi). Now, from Equation 6.1 F A 0 b 2 in which b is the crosssection side length. Thus, F ( N/m 2 )( m) N (1366 lb f ) (b) After the load is released there will be no deformation since the material was strained only elastically.
10 Question 6.29: A cylindrical specimen of aluminum having a diameter of in. (12.8 mm) and a gauge length of in. ( mm) is pulled in tension. Use the load elongation characteristics tabulated below to complete parts (a) through (f). Load Length N lb f mm in ,330 1, ,100 3, ,100 5, ,400 6, ,400 7, ,400 8, ,300 9, ,800 10, ,200 10, ,300 10, ,500 10, ,100 10, ,800 10, ,600 9, ,400 8, Fracture (a) Plot the data as engineering stress versus engineering strain. (b) Compute the modulus of elasticity. (c) Determine the yield strength at a strain offset of (d) Determine the tensile strength of this alloy. (e) What is the approximate ductility, in percent elongation? (f) Compute the modulus of resilience. This problem calls for us to make a stressstrain plot for aluminum, given its tensile loadlength data, and then to determine some of its mechanical characteristics.
11 (a) The data are plotted below on two plots: the first corresponds to the entire stressstrain curve, while for the second, the curve extends to just beyond the elastic region of deformation. (b) The elastic modulus is the slope in the linear elastic region (Equation 6.10) as E 200 MPa 0 MPa MPa 62.5 GPa ( psi)
12 (c) For the yield strength, the strain offset line is drawn dashed. It intersects the stressstrain curve at approximately 285 MPa (41,000 psi ). (d) The tensile strength is approximately 370 MPa (54,000 psi), corresponding to the maximum stress on the complete stressstrain plot. (e) The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by onehundred. The total fracture strain at fracture is 0.165; subtracting out the elastic strain (which is about 0.005) leaves a plastic strain of Thus, the ductility is about 16%EL. (f) From Equation 6.14, the modulus of resilience is just U r y 2 2E which, using data computed above gives a value of U r (285 MPa) 2 (2)( MPa) 0.65 MN/m N/m J/m 3 (93.8 in. lb f /in. 3 ) Question 6.40: Demonstrate that Equation 6.16, the expression defining true strain, may also be represented by T ln when specimen volume remains constant during deformation. Which of these two expressions is more valid during necking? Why? This problem asks us to demonstrate that true strain may also be represented by A 0 A i T ln A 0 A i Rearrangement of Equation 6.17 leads to
13 l i l 0 A 0 A i Thus, Equation 6.16 takes the form T ln l i l 0 ln A 0 A i The expression T ln A 0 A i is more valid during necking because A i is taken as the area of the neck. Question 6.44: The following true stresses produce the corresponding true plastic strains for a brass alloy: True Stress (psi) True Strain 50, , What true stress is necessary to produce a true plastic strain of 0.25? For this problem, we are given two values of T and T, from which we are asked to calculate the true stress which produces a true plastic strain of Employing Equation 6.19, we may set up two simultaneous equations with two unknowns (the unknowns being K and n), as log (50,000 psi) log K + n log (0.10) log (60,000 psi) log K + n log (0.20) Solving for n from these two expressions yields n log (50,000) log (60,000) log (0.10) log (0.20) and for K
14 log K 4.96 or K ,623 psi Thus, for T 0.25 T K ( T ) n (91,623 psi)(0.25) ,700 psi (440 MPa) Question 6.46: Find the toughness (or energy to cause fracture) for a metal that experiences both elastic and plastic deformation. Assume Equation 6.5 for elastic deformation, that the modulus of elasticity is 172 GPa ( psi), and that elastic deformation terminates at a strain of For plastic deformation, assume that the relationship between stress and strain is described by Equation 6.19, in which the values for K and n are 6900 MPa ( psi) and 0.30, respectively. Furthermore, plastic deformation occurs between strain values of 0.01 and 0.75, at which point fracture occurs. This problem calls for us to compute the toughness (or energy to cause fracture). The easiest way to do this is to integrate both elastic and plastic regions, and then add them together. Toughness d 0.01 E d + K n d E K 0.75 (n 1) (n 1) N/m 2 2 (0.01) N/m 2 ( ) (0.75) 1.3 (0.01) J/m 3 ( in.lb f /in. 3 ) Question 6.49: A cylindrical specimen of a brass alloy 7.5 mm (0.30 in.) in diameter and 90.0 mm (3.54 in.) long is pulled in tension with a force of 6000 N (1350 lb f ); the force is subsequently released.
15 (a) Compute the final length of the specimen at this time. The tensile stress strain behavior for this alloy is shown in Figure (b) Compute the final specimen length when the load is increased to 16,500 N (3700 lb f ) and then released. (a) In order to determine the final length of the brass specimen when the load is released, it first becomes necessary to compute the applied stress using Equation 6.1; thus F A 0 F d N m MPa (19,000 psi) Upon locating this point on the stressstrain curve (Figure 6.12), we note that it is in the linear, elastic region; therefore, when the load is released the specimen will return to its original length of 90 mm (3.54 in.). (b) In this portion of the problem we are asked to calculate the final length, after load release, when the load is increased to 16,500 N (3700 lb f ). Again, computing the stress 16,500 N m MPa (52,300 psi) The point on the stressstrain curve corresponding to this stress is in the plastic region. We are able to estimate the amount of permanent strain by drawing a straight line parallel to the linear elastic region; this line intersects the strain axis at a strain of about 0.08 which is the amount of plastic strain. The final specimen length l i may be determined from a rearranged form of Equation 6.2 as l i l 0 (1 + ) (90 mm)( ) mm (3.82 in.) Question 6.D1: A large tower is to be supported by a series of steel wires. It is estimated that the load on each wire will be 11,100 N (2500 lb f ). Determine the minimum required wire diameter assuming a factor of safety of 2 and a yield strength of 1030 MPa (150,000 psi).
16 For this problem the working stress is computed using Equation 6.24 with N 2, as w y MPa MPa (75,000 psi ) Since the force is given, the area may be determined from Equation 6.1, and subsequently the original diameter d 0 may be calculated as A 0 F d 2 0 w 2 And d 0 4F w (4)(11,100 N) ( N/m 2 ) m 5.23 mm (0.206 in.) Question 6.D2: (a) Gaseous hydrogen at a constant pressure of MPa (10 atm) is to flow within the inside of a thinwalled cylindrical tube of nickel that has a radius of 0.1 m. The temperature of the tube is to be 300 C and the pressure of hydrogen outside of the tube will be maintained at MPa (0.1 atm). Calculate the minimum wall thickness if the diffusion flux is to be no greater than mol/m 2 s. The concentration of hydrogen in the nickel, C H (in moles hydrogen per m 3 of Ni) is a function of hydrogen pressure, P H2 (in MPa) and absolute temperature (T) according to 12.3 kj/mol C H 30.8 p H2 exp (6.28) RT Furthermore, the diffusion coefficient for the diffusion of H in Ni depends on temperature as D H exp kj/mol RT (6.29)
17 (b) For thinwalled cylindrical tubes that are pressurized, the circumferential stress is a function of the pressure difference across the wall (Δp), cylinder radius (r), and tube thickness (Δx) as r p 4 x (6.30) Compute the circumferential stress to which the walls of this pressurized cylinder are exposed. (c) The roomtemperature yield strength of Ni is 100 MPa (15,000 psi) and, furthermore, s y diminishes about 5 MPa for every 50 C rise in temperature. Would you expect the wall thickness computed in part (b) to be suitable for this Ni cylinder at 300 C? Why or why not? (d) If this thickness is found to be suitable, compute the minimum thickness that could be used without any deformation of the tube walls. How much would the diffusion flux increase with this reduction in thickness? On the other hand, if the thickness determined in part (c) is found to be unsuitable, then specify a minimum thickness that you would use. In this case, how much of a diminishment in diffusion flux would result? (a) This portion of the problem asks for us to compute the wall thickness of a thinwalled cylindrical Ni tube at 300 C through which hydrogen gas diffuses. The inside and outside pressures are, respectively, and MPa, and the diffusion flux is to be no greater than mol/m 2 s. This is a steadystate diffusion problem, which necessitates that we employ Equation 5.3. The concentrations at the inside and outside wall faces may be determined using Equation 6.28, and, furthermore, the diffusion coefficient is computed using Equation Solving for x (using Equation 5.3) x D C J mol/m 2 s ( ,560 J /mol ) exp (8.31 J/mol K)( K) 12, 300 J/mol (30.8) exp MPa MPa (8.31 J/mol K)( K)
18 m 2.5 mm (b) Now we are asked to determine the circumferential stress: r p 4 x (0.10 m)(1.013 MPa MPa) (4)( m) 10.0 MPa (c) Now we are to compare this value of stress to the yield strength of Ni at 300 C, from which it is possible to determine whether or not the 2.5 mm wall thickness is suitable. From the information given in the problem, we may write an equation for the dependence of yield strength ( y ) on temperature (T) as follows: y 100 MPa 5 MPa 50 C T T r where T r is room temperature and for temperature in degrees Celsius. Thus, at 300 C y 100 MPa (0.1 MPa/ C) (300 C 20 C) 72 MPa Inasmuch as the circumferential stress (10 MPa) is much less than the yield strength (72 MPa), this thickness is entirely suitable. (d) And, finally, this part of the problem asks that we specify how much this thickness may be reduced and still retain a safe design. Let us use a working stress by dividing the yield stress by a factor of safety, according to Equation On the basis of our experience, let us use a value of 2.0 for N. Thus w y N 72 MPa 2 36 MPa Using this value for w and Equation 6.30, we now compute the tube thickness as
19 x r p 4 w (0.10 m)(1.013 MPa MPa) 4(36 MPa) m 0.70 mm Substitution of this value into Fick's first law we calculate the diffusion flux as follows: J D C x ( , 560 J/mol ) exp (8.31 J/mol K)( K) 12,300 J /mol (30.8) exp (8.31 J/mol K)( K) MPa MPa m mol/m 2 s Thus, the flux increases by approximately a factor of 3.5, from to mol/m 2 s with this reduction in thickness.
MAE 20 Winter 2011 Assignment 5
MAE 20 Winter 2011 Assignment 5 6.7 For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa (16.7 10 6 psi). (a) What is the
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationThere are three principle ways a load can be applied:
MATERIALS SCIENCE Concepts of Stress and Strains Stressstrain test is used to determine the mechanical behavior by applying a static load uniformly over a cross section or a surface of a member. The test
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationMECHANICAL PROPERTIES OF MATERIALS. IE114 Materials Science and General Chemistry Lecture6
MECHANICAL PROPERTIES OF MATERIALS IE114 Materials Science and General Chemistry Lecture6 Overview 1) ELASTIC DEFORMATION  Elastic Behavior  Anelasticity  Elastic Properties of Materials 2) PLASTIC
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationME 105 Mechanical Engineering Laboratory Spring Quarter Tensile Test
ME 105 Mechanical Engineering Lab Page 1 ME 105 Mechanical Engineering Laboratory Spring Quarter 2003 3. Tensile Test Introduction In this lab, you will study the deformation and fracture characteristics
More informationMSE 527L  Testing of Materials in Tension
MSE 527L  Testing of Materials in Tension Object: The object of this experiment is to measure the tensile properties of steel, copper and aluminum at a constant strain rate on the tension testing machine
More informationStructures and Stiffness
Structures and Stiffness ENGR 10 Introduction to Engineering Ken Youssefi/Thalia Anagnos Engineering 10, SJSU 1 Wind Turbine Structure The Goal The support structure should be optimized for weight and
More informationStressStrain Relationship
(Strength of Materials) Dave Morgan StressStrain Relationship p. 1/21 The tension test: StressStrain Relationship p. 2/21 The tension test: Is a common standardised test that can
More informationPrinciples of Fracture Mechanics
81 CHAPTER 8 FAILURE PROBLEM SOLUTIONS Principles of Fracture Mechanics 8.1 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an internal crack. Equation
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationBEYOND ELASTICITY. Subtopics. Plasticity Toughness Hardness Design problems
BEYOND ELASTICITY Subtopics 1 Plasticity Toughness Hardness Design problems PLASTICITY The stress is no longer proportional to strain 2 STRESSSTRAIN BEHAVIOR: PLASTICITY Tensile strength is the stress
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationMSE200 Lecture 7 (CH ) Mechanical Properties I Instructor: Yuntian Zhu Objectives/outcomes: You will learn the following:
MSE200 Lecture 7 (CH. 6.26.4) Mechanical Properties I Instructor: Yuntian Zhu Objectives/outcomes: You will learn the following: Stresses and strains in solids. Normal and shear stresses. Elastic and
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationProblem P5.2: A 1 Mg container hangs from a 15 mm diameter steel cable. What is the stress in the cable?
Problem P5.: A 1 Mg container hangs from a 15 mm diameter steel cable. What is the stress in the cable? Find the cross sectional area in terms of diameter using Equation (5.1). Calculate the tensile stress
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationStatics and Mechanics of Materials
Statics and Mechanics of Materials Chapter 4 Stress, Strain and Deformation: Axial Loading Objectives: Learn and understand the concepts of internal forces, stresses, and strains Learn and understand the
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationChapter 4 Strain and Material Relations
CIVL 222 STRENGTH OF MATERIALS Chapter 4 Strain and Material Relations Terminology 1. Displacement 2. Deformation 3. Strain 4. Average Axial Strain 5. Shearing Strain 6. Poisson s Ratio 7. Mechanical Properties
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationσ y ( ε f, σ f ) ( ε f
Typical stressstrain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A =  A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
More informationPLASTIC DEFORMATION AND STRESSSTRAIN CURVES
PLASTIC DEFORMATION AND STRESSSTRAIN CURVES Introduction Background Unit: Plastic Deformation and StressStrain Curves In the last unit we studied the elastic response of materials to externally applied
More informationSAMPLE OF THE STUDY MATERIAL PART OF CHAPTER 1 STRESS AND STRAIN
SAMPLE OF THE STUDY MATERIAL PART OF CHAPTER 1 STRESS AND STRAIN 1.1 Stress & Strain Stress is the internal resistance offered by the body per unit area. Stress is represented as force per unit area. Typical
More informationPlastic Behaviour  Tensile Strength
Plastic Behaviour  Tensile Strength Transition of mechanical behaviour from elastic to plastic depends upon the material type and its condition as tested (hotrolled, coldrolled, heat treated, etc.).
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationSAMPLE OF THE STUDY MATERIAL PART OF CHAPTER 1 STRESS AND STRAIN
1.1 Stress & Strain SAMPLE OF THE STUDY MATERIAL PART OF CHAPTER 1 STRESS AND STRAIN Stress is the internal resistance offered by the body per unit area. Stress is represented as force per unit area. Typical
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationMCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions
MCEN 2024, Spring 2008 The week of Apr 07 HW 9 with Solutions The Quiz questions based upon HW9 will open on Thursday, Apr. 11 and close on Wednesday, Apr 17 at 1:30 PM. References to A&J: Chapters 13,
More informationTensile Testing of Steel
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0  INTRODUCTION See General Lab Report Format
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationPin jointed structures are often used because they are simple to design, relatively inexpensive to make, easy to construct, and easy to modify.
4. FORCES in PIN JOINTED STRUCTURES Pin jointed structures are often used because they are simple to design, relatively inexpensive to make, easy to construct, and easy to modify. They can be fixed structures
More informationME 215 Engineering Materials I
ME 215 Engineering Materials I Chapter 3 Properties in Tension and Compression (Part III) Mechanical Engineering University of Gaziantep Dr. A. Tolga Bozdana www.gantep.edu.tr/~bozdana True Stress and
More informationReview from Mechanical Properties of Materials
Fall 24 Review from Mechanical Properties of Materials Concept of Stress and Strain Figure 1 shows the behavior of a clindrical bod subjected to tension and compression. Tension specimen etends along its
More informationStrength and Stiffness
Strength and Stiffness Stress = load/area is applied to a material by loading it Strain = deformation/length a change of shape (dimensions and twist angles) is its response Stiffness = stress/strain is
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationCHAPTER 4 TENSILE TESTING
CHAPTER 4 TENSILE TESTING EXERCISE 28, Page 7 1. What is a tensile test? Make a sketch of a typical load/extension graph for a mild steel specimen to the point of fracture and mark on the sketch the following:
More informationMechanics of MaterialsSteel
Mechanics of MaterialsSteel Structural Steel Structural steel considered one of the predominant materials for construction of buildings, bridges, towers and other structures. The preferable physical properties
More informationWelcome to the first lesson of third module which is on thinwalled pressure vessels part one which is on the application of stress and strain.
Strength of Materials Prof S. K. Bhattacharya Department of Civil Engineering Indian Institute of Technology, Kharagpur Lecture 15 Application of Stress by Strain Thinwalled Pressure Vessels  I Welcome
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationSection 1: THE TEST CERTIFICATE
Section 1: THE TEST CERTIFICATE The objective of Section 1 is to explain the Metallurgical makeup of the Material Test Certificate. Introduction A material test certificate is used to report the chemical
More informationMaterial Types and Properties
Material Types and Properties 1 Material Types There are many kinds of materials, but most of them can be divided into four groups: Metals  Metals are composed of one or more metallic elements and often
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationTENSILE TESTING PRACTICAL
TENSILE TESTING PRACTICAL MTK 2B Science Of Materials Ts epo Mputsoe 215024596 Summary Material have different properties all varying form mechanical to chemical properties. Taking special interest in
More informationStrength of materials
Strength of materials 1. General concepts All structures, both natural and manmade, are composed of materials that are arranged and assembled in a way that will fulfill the purpose of the structure. Buildings,
More informationChapter 12 Elasticity
If I have seen further than other men, it is because I stood on the shoulders of giants. Isaac Newton 12.1 The Atomic Nature of Elasticity Elasticity is that property of a body by which it experiences
More informationSTRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION
Chapter 11 STRESS AND DEFORMATION ANALYSIS OF LINEAR ELASTIC BARS IN TENSION Figure 11.1: In Chapter10, the equilibrium, kinematic and constitutive equations for a general threedimensional solid deformable
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationStrength of materials
Strength of materials 1. General concepts All structures, both natural and manmade, are composed of materials that are arranged and assembled in a way that will fulfill the purpose of the structure. Buildings,
More informationStrength of Materials
Strength of Materials 1. Strain is defined as the ratio of (a) change in volume to original volume (b) change in length to original length (c) change in crosssectional area to original crosssectional
More informationM n = (DP)m = (25,000)(104.14 g/mol) = 2.60! 10 6 g/mol
14.4 (a) Compute the repeat unit molecular weight of polystyrene. (b) Compute the numberaverage molecular weight for a polystyrene for which the degree of polymerization is 25,000. (a) The repeat unit
More informationProperties of Matter
Mr. Patrick J Camilleri B.Ed (Hons) M.Ed Science (Sheffield) Department of Physics JC Malta Properties of Matter Basics You Should Know Elasticity. Young modulus 1. Hooke's law. Extension α tension (force
More informationMechanical properties laboratory practice guide 2015
Mechanical properties laboratory practice guide 215 Hardness test methods Hardness is resistance of material to plastic deformation caused by indentation. 1. Brinell Hardness Test [1] Dr. J. A. Brinell
More informationExperiment: Mechanical Testing Tensile Testing
Experiment: Mechanical Testing Tensile Testing Objective The primary objective of this investigation is to conduct a standard tensile test for determining the stressstrain behavior of a material sample
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. UNIT I STRESS STRAIN DEFORMATION OF SOLIDS PART A (2 Marks)
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK SUB CODE/NAME: CE1259 STRENGTH OF MATERIALS YEAR/SEM: II / IV 1. What is Hooke s Law? 2. What are the Elastic Constants?
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 1 STRESSES IN BEAMS DUE TO BENDING. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS  BEAMS TUTOIAL 1 STESSES IN BEAMS DUE TO BENDING This is the first tutorial on bending of beams designed for anyone wishing to study it at a fairly advanced level. You should judge
More informationCHAPTER 9 : MECHANICAL PROPERTIES OF SOLIDS ONE MARK QUESTIONS: 1. What is elasticity of a body? 2. What is plasticity? 3. Which property of a body
1 CHAPTER 9 : MECHANICAL PROPERTIES OF SOLIDS ONE MARK QUESTIONS: 1. What is elasticity of a body? 2. What is plasticity? 3. Which property of a body is responsible for regaining original shape and size
More informationSTRESSSTRAIN RELATIONS
STRSSSTRAIN RLATIONS Strain Strain is related to change in dimensions and shape of a material. The most elementar definition of strain is when the deformation is along one ais: change in length strain
More informationFor Cu, which has an FCC crystal structure, R = nm (Table 3.1) and a = 2R 2 =
7.9 Equations 7.1a and 7.1b, expressions for Burgers vectors for FCC and BCC crstal structures, are of the form a b = uvw where a is the unit cell edge length. Also, since the magnitudes of these Burgers
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
CHAPTER 8 DEFORMATION AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 8.1 To provide some perspective on the dimensions of atomic defects,
More informationMATERIALS SCIENCE AND ENGINEERING
Complete Solutions to Selected Problems to accompany MATERIALS SCIENCE AND ENGINEERING AN INTRODUCTION Sixth Edition William D. Callister, Jr. The University of Utah John Wiley & Sons, Inc. Copyright 2003
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationStress and Strain Elasticity
Stress and Strain Elasticit Notation: A = area D = diameter dimension E = modulus of elasticit or Young s modulus f = stress F allow. = allowable stress F t = allowable tensile stress F.S. = factor of
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationBending Beam. Louisiana State University. Joshua Board
Bending Beam Louisiana State University Joshua Board Table of Contents: Table of Figures:... 4 Purpose... 5 Introduction... 5 Apparatus and Test Procedures... 11 Summary of Data... 14 Discussion of Results...
More informationME 388 APPLIED INSTUMENTATION LAB Mechanical Properties by Tensile Testing
1 Prepared 6/27/08 by Dr. Kraft Learning Objectives 1. To learn fundamentals of tensile testing to determine basic mechanical properties of materials. 2. To analyze tensile test data to analytically model
More informationMechanics of Materials
Mechanics of Materials Notation: a = acceleration A = area (net = with holes, bearing = in contact, etc...) ASD = allowable stress design d = diameter of a hole = calculus symbol for differentiation e
More information1. Steel fasteners for the temperature range between 50 C and +150 C
1. Steel fasteners for the temperature range between 50 C and +150 C 1.1 Materials for fasteners The material that is used is of decisive importance for the quality of the fasteners (screws, nuts and fittings).
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationMECHANICS OF MATERIALS
CHAPTER 2 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Lecture Notes: J. Walt Oler Texas Tech University Stress and Strain Axial Loading Normal Strain
More informationCH 4: Deflection and Stiffness
CH 4: Deflection and Stiffness Stress analyses are done to ensure that machine elements will not fail due to stress levels exceeding the allowable values. However, since we are dealing with deformable
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationCHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS
191 CHAPTER 19 THERMAL PROPERTIES PROBLEM SOLUTIONS Heat Capacity 19.1 The energy, E, required to raise the temperature of a given mass of material, m, is the product of the specific heat, the mass of
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationSolution: The draft attempted in this rolling operation is
Example: 1 A 300mmwide strip 25 mm thick is fed through a rolling mill with two powered rolls each of radius = 250 mm. The work thickness is to be reduced to 22 mm in one pass at a roll speed of 50 rev/min.
More informationInteraction of Hydrogen and Deformation in 316L Stainless Steel
Proceedings of the SEM Annual Conference June 14, 2009 Albuquerque New Mexico USA 2009 Society for Experimental Mechanics Inc. Interaction of Hydrogen and Deformation in 316L Stainless Steel Bonnie R.
More informationCHAPTER 2 ATOMIC STRUCTURE AND INTERATOMIC BONDING PROBLEM SOLUTIONS
CHPTER 2 TOMIC STRUCTURE ND INTERTOMIC BONDING PROBLEM SOLUTIONS 2.2 Chromium has four naturallyoccurring isotopes: 4.34% of 50 Cr, with an atomic weight of 49.9460 amu, 83.79% of 52 Cr, with an atomic
More informationTensile Testing of Nanoscale and Macroscale Metal Samples
Tensile Testing of Nanoscale and Macroscale Metal Samples Instructions and Safety: Please read this lab handout and the required background reading before the Monday prelab lecture. You should also review
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationMechanical properties 3 Bend test and hardness test of materials
MME131: Lecture 15 Mechanical properties 3 Bend test and hardness test of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Bend test of brittle materials Hardness testing
More informationCourse 1 Laboratory. Second Semester. Experiment: Young s Modulus
Course 1 Laboratory Second Semester Experiment: Young s Modulus 1 Elasticity Measurements: Young Modulus Of Brass 1 Aims of the Experiment The aim of this experiment is to measure the elastic modulus with
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationStrength of Materials
FE Review Strength of Materials Problem Statements Copyright 2008 C. F. Zorowski NC State E490 Mechanics of Solids 110 KN 90 KN 13.5 KN A 3 = 4.5x103 m 2 A 2 = 2x103 m 2 A 1 = 5x104 m 2 1. A circular
More informationTHE WAY TO SOMEWHERE. Subtopics. Diffusion Diffusion processes in industry
THE WAY TO SOMEWHERE Subtopics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
More informationMATERIALS SELECTION FOR SPECIFIC USE
MATERIALS SELECTION FOR SPECIFIC USE1 Subtopics 1 Density What determines density and stiffness? Material properties chart Design problems LOADING 2 STRENGTH AND STIFFNESS Stress is applied to a material
More informationPhysics 3 Summer 1989 Lab 7  Elasticity
Physics 3 Summer 1989 Lab 7  Elasticity Theory All materials deform to some extent when subjected to a stress (a force per unit area). Elastic materials have internal forces which restore the size and
More informationREINFORCED CONCRETE. Reinforced Concrete Design. A Fundamental Approach  Fifth Edition
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition CONCRETE Fifth Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More information